IOSR Journal of Engineering (IOSRJEN) e-ISSN: 2250-3021, p-ISSN: 2278-8719, www.iosrjen.org Volume 2, Issue 10 (October 2012), PP 07-11
Engineering Properties of Cement CONTAINING POND ASH Milind P. Bhamare1, Yogesh N. Bafna2, Arun K. Dwivedi3
Abstract: A thermal power plants converts energy rich fuel into electricity and heat. Coal produced electricity takes about 80 % of the total power generated in India. The coal based power plant generates a huge amount of ash. The generated ash contains about 20 percent Pond ash and 80 percent fly ash of the total ash generated. Fly ash is been recycled as an alternative to cement while pond ash is being disposed off. Pond ash requires huge area , water and energy to dispose itself off so recycling of the pond ash is indeed required. This paper concentrates on utilization of pond ash as a cement replacement.
A thermal power plants converts energy rich fuel into electricity and heat. The fuel includes coal, natural gases, petroleum products, agriculture waste and domestic trash/waste, landfill gas and biogas etc. Coal and liginte accounts for about 57% of India’s installed capacity of power generation. Coal produced electricity takes about 80 % of the total power generated in India. The Indian power plant uses coal like Gondwana coal; it has low calorific value and high ash content which requires 0.7 kg of coal to generate a 1 kwh of electricity. The coal based power plant generates a huge amount of ash. In India, it is about 170 MT for the year 2011-12 and is expected to be above 600MT for the year 2031-32. The generated ash contains about 20 percent Pond ash and 80 percent fly ash of the total ash generated. Fly ash is been recycled as an alternative to cement while pond ash is being disposed off. The disposal of large quantity of pond ash requires huge area of land, water and energy. If not managed well becomes a health hazard and damages the environment. With increased power consumption the generation of coal ash has been growing annually and need for additional disposal sites has become urgent. So recycling pond ash might be able to sort out the above mentioned issues. This paper addresses the issues pertaining to the change in engineering properties of the cement containing pond ash.
2.1 MATERIALSExperimentations have been on 53 grade OPC cement to find out its physical and chemical properties. The physical and chemical properties of OPC cement used for the research work are shown in the Table 1 and 2. Pond ash used for the cement replacement is collected from the thermal power plant situated at Deepnagar, Bhusawal, Maharashtra. Quartzanium TM Sand (standard sand) used as fine aggregate, for research work. Properties of pond ash and standard sand are given in Table 3 and 4. Figure 1 shows the grain size distribution of pond ash. It is observed that 66 percent of Total weight of the pond ash is smaller than 0.075mm. Fineness modulus is 1.656
Type of Cement OPC(53 Grade) (IS 122691987)
Table 1. Chemical Characteristics of Cement. Lime Alumina Insoluble Magnesia Sulphuric Saturation Iron Ratio Residue (%) Max. Anhydride Factor (%) (%) Min. (%) Max. 0.8 Min., 1.02 Max.
Loss on Ignition (%) Max. 4
Table 2 “Physical Characteristics of Cement.” Type of Cement OPC(53 Grade) (IS 122691987)
Setting Time Initial (mins)
Compressive Strength 3 Days N/mm2
7 Days N/mm2
Engineering Properties of Cement CONTAINING POND ASH Table 3 â€œPhysical and Chemical Characteristics of Standard sand.â€? Quartzanium TM Sand Properties (Standard Sand) Physical Properties Color Whitish Specific Gravity 2.65 W. Absorption in 24 hours 0.30% Shape of Grains Sub Angular Chemical Properties SiO2 99.42% Al2O3 0.18% Fe2O3 0.02% CaO Loss on Ignition 0.10% Table 4 Physical Properties of Pond Ash Properties Pond Ash Physical Properties Color Whitish grey Specific Gravity 2.153 W. Absorption in 24 hours 44.50%
Fig. 1 particle size distribution curve f Pond ash 100 90 80 70 60 50 40 30 20 10 0 0.1
1 Particle Size (mm)
2.2 Mix Proportions As a replacement of cement, pond ash is mix in different percentage. The percentage and mix proportions are given in the Table 5.
Sr. No 1
Table 5 Cement labels and mix proportions Mix proportion Quantity of material (kg) Description and Label Pond C:PA:S Cement Sand ash OPC OPC including 0.0% of pond ash by mass of 2.22 0 6.66 cement as replacement of cement (OPC) 1:00:03 M1
OPC including 2.5% of pond ash by mass of cement as replacement of cement (M 1)
OPC including 5.0% of pond ash by mass of
Engineering Properties of Cement CONTAINING POND ASH cement as replacement of cement (M 2)
OPC including 7.5% of pond ash by mass of cement as replacement of cement (M 3)
OPC including 10.0% of pond ash by mass of cement as replacement of cement (M 4)
OPC including 12.5% of pond ash by mass of cement as replacement of cement (M 5)
OPC including 15.0% of pond ash by mass of cement as replacement of cement ((M 6))
OPC including 17.5% of pond ash by mass of cement as replacement of cement ((M 7)
OPC including 20.0% of pond ash by mass of cement as replacement of cement (M 8)
OPC including 22.5% of pond ash by mass of cement as replacement of cement (M 9)
0.925:0.075:3 M4 M5 M 6 0.85:0.15:3 M7 0.825:0.175:3 M8 0.8:0.2:3 M9 0.775:0.225:3
2.3 Test methods Materials used in this research work are an OPC cement, pond ash and fine aggregate, Materials are tested as per Indian standard and mention in the Table 6 below. Table 6 Standard utilized for testing Test Method Normal Consistency Setting Time La Chatelier Tests Performed on Cement Mortar Compressive Strength
Related Standard I.S.4031- (Part 4) 1988 I.S.4031-(Part 5) 1988 IS : 4031-(Part 3) 1988 IS : 4031-(Part 6) 1988
Test results and discussions
3.1 Analysis of the properties of cement 3.1.1 Normal consistency of cement- I.S.4031- (Part 4) 1988 The test results are shown in Table 7. Due to the porous nature of the pond ash particles, requires more water to make a plastic cement paste compare to ordinary Portland cement. It is observed that an amount of water required to make a plastic cement paste goes on increasing with the percentage content of the pond ash in cement.
Cement OPC M1 M2 M3 M4 M5 M6 M7 M8 M9
Table 7. Normal Consistency Result of Cement Pastes Required Amount of water for Normal Consistency % of Pond Ash % gm 0.0 30.0 90.0 2.5 31.8 95.4 5.0 32.9 98.7 7.5 33.6 100.8 10.0 34.7 104.1 12.5 35.8 107.4 15.0 37.9 113.7 17.5 39.4 118.2 20.0 40.8 122.4 22.5 42.1 126.3
Engineering Properties of Cement CONTAINING POND ASH 3.1.2 Setting Time For ease of construction the initial setting must not be too short and final setting must not be too long. Table 8 shows the initial and final setting time values for ordinary Portland cement containing different percentage of pond ash. Initial and final setting time increases with the increase in the percentage of pond ash content in the cement. Increased time seen due to the less pozzolanic properties of pond ash.
Cement OPC M1 M2 M3 M4 M5 M6 M7 M8 M9
Percentage of Pond Ash 0 2.5 5 7.5 10 12.5 15 17.5 20 22.5
Table 8 Setting Time of Cement Initial Setting Time (min.) 52 55 60 68 73 78 84 88 94 102
Final Setting Time (min.) 290 302 308 319 328 345 357 373 386 395
3.1.3 Volume Expansion The test was conducted on 10 samples containing 0 to 22.5% of pond ash using le Chateliers soundness test. This test only takes into account CaO. Hydration product has larger volume than that of free time and finally gives rise to cracks. Thus, partly replaced pond ash give advantages volume expansion results due to lower free time value in cement paste.
Cement OPC M1 M2 M3 M4 M5 M6 M7 M8 M9
Table 9 Soundness test of Cement (Values are near to 0.5 mm) % of Pond Ash Change in distance (mm) 0 2.5 2.5 3.0 5 2.5 7.5 2.5 10 2.0 12.5 2.0 15 2.0 17.5 2.0 20 1.5 22.5 1.5
3.1.4 Compressive Strength of Cement The compressive strength of cement decreases with increase by the content of percentage pond ash. The growing content of pond ash is responsible for decrease in the compressive strength of cement. A mix of cement & pond ash has less compressive strength as compared to the OPC as pond ash contains both fine as well as non reactive large particle due to which it has less pozzolanic property. Graph 2 Compressive strength of cement
10 | P a g e
Compressive Strength (Mpa)
Engineering Properties of Cement CONTAINING POND ASH
70 60 50 40 30 20 10 0
M1 M2 M3 M4 M5 M6 M7
Mix M1 M2 M3 M4 M5 M6 M7 M8 M9
Table 10 percentage compressive strength of pond as incorporated cement w. r. t. OPC Percentage compressive strength % P.A. 3 Days 7 Days 28 Days 42 Days 70 Days 92 Days 126 Days 2.5 93.889 97.919 98.755 97.745 95.491 96.914 98.525 5.0 92.704 96.946 97.453 96.127 94.509 94.707 97.780 7.5 92.074 95.216 95.774 93.400 92.596 92.810 94.373 10.0 90.481 93.703 92.415 91.145 90.649 91.569 93.441 12.5 87.667 94.946 89.377 88.964 88.193 88.707 90.288 15.0 84.926 93.189 87.264 87.036 84.947 85.638 87.915 17.5 81.904 91.000 86.358 84.000 82.877 83.690 85.186 20.0 79.074 88.595 83.623 82.036 81.825 82.534 83.627 22.5 75.741 84.351 79.509 77.582 77.193 77.810 80.254
The results of the basic study to utilize pond ash as cement replacement and change in engineering properties of cement containing pond ash are as under. 1) Pond ash should be utilized by identifying its qualities which greatly depends on the particle sizes. 2) From the examination on pond ash used for cement replacement it can be inferred that the normal consistency of cement defer according to the percentage pond ash. 3) From the examination on the pond ash incorporated cement, it can be inferred that the pond ash acts as retarder & increases the initial setting time of the cement paste. 4) It is observed from the analysis of the compressive strength results that as the pond ash percentage increases in the cement paste the compressive strength decreases due to low pozzolanic property of the pond ash.
Reference        
Bera, Ghosh & Ghosh (2007), “Compaction Characteristics of Pond Ash”, Journal - Materials in Civil Engineering, Volume IXX, Issue-4, April-2007, pp-349-357. Cheriaf M., Cavalcante Rocha, J., Pérab, J. (1999). Pozzolanic properties of pulverized coal combustion bottom ash. Cement and Concrete Research, 29, 1387–1391. IS 4031 –Testing of Cement. Halstead, W.J. (1986). Use of fly ash in concrete. Washington, DC: Transportation Research Board. Jaturapitakkul, C., Cheerarot, R. (2003). Development of bottom ash as pozzolanic material. Journal of Materials in Civil Engineering, 15, 48-53. Lee, S. H., Hong J. K., Sakai, E., Daimon, M. (2003). Effect of particle size distribution of fly ash–cement system on the fluidity of cement pastes. Cement and Concrete Research , 33, 763–768. Mangaraj & Krishnamoorthy (1994), “Use of Ponded Flyash as part Replacement of fine Aggregate in Mortar and Concrete”, The Indian Concrete Journal, May-1994, pp-279-282. Ritwik, Singh & Das (2001), “Effect of Addition of Pond Ash and Fly ash on properties of Ash-Clay Burnt Bricks”, Journal - Waste Management & Research, ISSN 0734–242X, 2007: 25 : pp- 566–571.
11 | P a g e
Published on Dec 25, 2012